Kielce University of Technology, Faculty of Mechatronics and Machine Design, Kielce, Poland


 Miles Conley
 1 years ago
 Views:
Transcription
1 JOURNAL OF THEORETICAL AND APPLIED MECHANICS 50,1,pp.2346,Warsaw th anniversary of JTAM THE INFLUENCE OF MATERIAL PROPERTIES AND CRACK LENGTHONTHEQSTRESSVALUENEARTHECRACKTIP FOR ELASTICPLASTIC MATERIALS FOR CENTRALLY CRACKED PLATE IN TENSION Marcin Graba Kielce University of Technology, Faculty of Mechatronics and Machine Design, Kielce, Poland In the paper, values of the Qstress determined for various elasticplastic materials for centre cracked plate in tension(cc(t)) are presented. The influence of the yield strength, the workhardening exponent and the crack length on the Qparameter was tested. The numerical results were approximated by closed form formulas. This paper is a continuation of the catalogue of the numerical solutions presented in 2008, which presents Qstress solutions for single edge notch specimens in bending SEN(B). Both papers present full numerical results and their approximationfortwobasicspecimenswhichareusedtodetermineinthelaboratory tests the fracture toughness Jintegral, and both specimens are proposed by FITNET procedure used to idealize the real components. Key words: fracture mechanics, cracks, Qstress, stress fields, HRR solution, FEM, Jintegral, O Dowd theory 1. Introduction theoretical backgrounds about JQ theory The stress field near crack tip for the nonlinear RambergOsgood(RO) material was described in 1968 by Hutchinsonson, who published the fundamental work for fracture mechanics. The presented by Hutchinson solution, now called thehrrsolution,includesthefirsttermoftheinfiniteseriesonly.the numerical analysis shows that the results obtained using the HRR solution are different from the results obtained using the finite element method FEM (Fig.1).Toeliminatethisdifference,itisnecessarytousemoretermsinthe HRR solution.
2 24 M. Graba Fig.1.ComparisonofFEMresultsandHRRsolutionfortheplanestressandplane strain for a single edge notched specimen in bending(sen(b)) and centrally cracked plateintension(cc(t));e=206000mpa,n=5,ν=0.3,σ 0 =315MPa, ε 0 =σ 0 /E= ,a/W=0.50,W=40mm,θ=0 FirstitwasdonebyLiandWang(1985),whousingtwotermsinthe Airy function, obtained the second term of the asymptotic expansion only fortwodifferentmaterials,describedbytheroexponentequalto n=3 and n=10.theiranalysisshowsthatthetwotermsolutionmuchbetter describesthestressfieldnearthecracktip,andthevalueofthesecondterm, which may not to be negligible depends on the material properties and the specimen geometry. AmoreaccuratesolutionwasproposedbyYangetal.(1993),whousingthe Airy function with the separate variables proposed that the stress field near the cracktipmaybedescribedbyaninfiniteseriesform.theproposedbythem solution is currently used with only three terms of the asymptotic solution, and itisoftencalled JA 2 theory.yangetal.(1993)conductedfulldiscussion about their idea. They showed that the multiterms description, which uses three terms of the asymptotic solution is better than the Hutchinson approach. TheA 2 amplitude,whichisusedintheja 2 theorysuggestedbyyangetal. (1993) is nearly independent of the distance of the determination, but using the JA 2 theoryinengineeringpracticeissometimesveryburdensome,because anengineermustknowthe σ (k) ij function and the power exponent t, which are to be calculated by solving a fourth order differential equation, and next usingfemresults,theengineermustcalculatethea 2 amplitude. The simplified solution for describing the stress field near the crack tip for elastic plastic materials was proposed by O Dowd and Shih(1991, 1992). ThatconceptwasdiscussedbyShihetal.(1993).TheyassumedthattheFEM results are exact and computed the difference between the numerical and HRR
3 The influence of material properties and crack length results. They proposed that the stress field near the crack tip may be described by the following equation ( J ) 1 ( n+1 r ) σ ij =σ 0 σ ij (θ,n)+σ 0 Q q σij (θ,n) (1.1) αε 0 σ 0 I n (n)r J/σ 0 whererandθarepolarcoordinatesofthecoordinatesystemlocatedatthe cracktip,σ ij arethecomponentsofthestresstensor,jisthejintegral,nis theroexponent,αistheroconstant,σ 0 theyieldstress,ε 0 strain relatedtoσ 0 throughε 0 =σ 0 /E, σ ij (θ;n)arefunctionsevaluatednumerically,qisthepowerexponentwhosevaluechangesintherange(0;0.071),and Qisaparameter,whichistheamplitudeofthesecondtermintheasymptotic solution.thefunctions σ ij (n,θ),i n (n)mustbefoundbysolvingthefourth order nonlinear homogenous differential equation independently for the plane stress and plane strain(hutchinson, 1968) or these functions may be found using the algorithm and computer code presented in Gałkiewicz and Graba (2006). O Dowd and Shih (1991, 1992) tested the Qparameter in the range J/σ 0 <r<5j/σ 0 nearthecracktip.theyshowed,thatthe Qparameter weaklydependsonthecracktipdistanceintherangeof±π/2.theyproposed onlytwotermstodescribethestressfieldnearthecracktip σ ij =(σ ij ) HRR +Qσ 0 σ ij (θ) (1.2) where(σ ij ) HRR (isthefirsttermofeq.(1.1)anditisthehrrsolution. To avoid the ambiguity during the calculation of the Qstress, O Dowd and Shih(1991, 1992) suggested that the Qstress should be computed at thedistancefromthecracktipwhichisequaltor=2j/σ 0 forthedirection θ=0.theypostulatedthatfortheθ=0directionthefunction σ θθ (θ=0) isequalto1.thatiswhytheqstressmaybecalculatedfromthefollowing relationship Q= (σ θθ) FEM (σ θθ ) HRR σ 0 forθ=0 and rσ 0 J =2 (1.3) where(σ θθ ) FEM isthestressvaluecalculatedusingfemand(σ θθ ) HRR isthe stress evaluated form the HRR solution(these are the opening crack tip stress components). During analysis, O Dowd and Shih(1991, 1992) showed that the Qstress value determines the level of the hydrostatic stress. For a plane stress, the Qparameterisequaltozerooritisclosetozero,butforaplanestrain,the Qparameter is in the most cases smaller than zero(fig. 2). The Qstress value foraplanestraindependsontheexternalloadinganddistancefromthecrack tip especially for large external loads(fig. 2b).
4 26 M. Graba Fig. 2. JQ trajectories measured at six distances near the crack tip for centrally cracked plate in tension(cc(t)):(a) plane stress,(b) plane strain(own calculation); W=40mm,a/W=0.5,σ 0 =315MPa,ν=0.3,E=206000MPa,n=5 2. Engineering aspects of JQ theory, fracture criteria based on the O Dowd approach UsingtheO DowdandShihtheorytodescribethestressfieldnearthecracktip for elasticplastic materials, the difference between the HRR solution(hutchnison, 1968) and the results obtained using the finite element method(fem) can be eliminated. O Dowd s theory is quite simple to use in practice, because inordertodescribethestressfieldnearthecracktip,wemustknowonlymaterial properties(yield stress, work hardening exponent), Jintegral and the Qstress value, which may be evaluated numerically or determined using the approximation presented in literature, for example Graba(2008). O Dowd s approachiseasierandmoreconvenienttouseincontrastto JA 2 theory, whichwasproposedbyyangetal.(1993).basedonthejqtheory,o Dowd (1995) proposed the following fracture criterion J C =J IC ( 1 Q σ c /σ 0 ) n+1 (2.1) wherej C istherealfracturetoughnessforastructuralelementcharacterised by a geometrical constraint defined by Qstress(whose value is usually is smallerthanzero),j IC isthefracturetoughnessfortheplanestraincondition for Q=0and σ c isthecriticalstressaccordingtotheritchieknottrice hypothesis(ritchie et al., 1973). Proposed by O Dowd fracture criterion was discussed by Neimitz et al. (2007), where the authors proposed another form. They modified O Dowd s
5 The influence of material properties and crack length formulas(eq.(2.1)),byreplacingthecriticalstressσ c bymaximumopening stressσ max,whichmustbeevaluatednumericallyusingthelargestrainformulation. The proposed by Neimitz et al.(2007) formulas have the following form Q ) n+1 J C =J IC (1 (2.2) σ max /σ 0 Forasingleedgenotchinbending(SEN(B)),Neimitzetal.(2007) using the finite element method and the large strain formulation estimated the maximumopeningstressσ max forseveralmaterials(differentroexponents, different yield stresses) and for several crack lengths. The JQ theory found application in European Engineering Programs, like SINTAP(1999) or FITNET(2006). The Qstresses are applied for construction of the fracture criterion and to assess the fracture toughness of structural components.therealfracturetoughness K C mat maybeevaluatedusingthe formula proposed by Ainsworth and O Dowd(1994). They showed that the increase in fracture in both the brittle and ductile regimes may be represented byanexpressionoftheform K C mat = { Kmat for βl r >0 K mat [1+α( βl r ) k ] for βl r <0 (2.3) wherek mat isthefracturetoughnessfortheplanestrainconditionobtained using FITNET procedures, and β is the parameter calculated using the following formula { T/(Lr σ 0 ) forelasticmaterials β= Q/L r forelasticplasticmaterials (2.4) where L r istheratiooftheactualexternalload P andthelimitload P 0 (or the reference stress), which may be calculated using FITNET procedures (FITNET, 2006). Theconstantsαandk,whichareoccurringinEq.(2.3),arematerialand temperature dependent(table 1). Sherry et al.(2005a,b) proposed procedures to calculate the constants α and k. Thus O Dowd s theory has practical application to engineering issues. Sometimes,theJQtheorymaybelimited,becausethereisnovalueofthe Qstress for a given material and specimen. Using any fracture criterion, for example that proposed by O Dowd(1995) or another one, Eq.(2.3)(FITNET, 2006)orthatpresentedbyNeimitzetal.(2007)(seeEq.(2.2)),orpresented by Neimitz et al.(2004), an engineer can estimate the fracture toughness quite fast, if the Qstress is known.
6 28 M. Graba Table1.SomevaluesoftheαandkparametersfromEq.(2.3)(SINTAP, 1999; FITNET, 2006) Material Temperature Fracture mode α k A533B(steel) 75 C cleavage A533B(steel) 90 C cleavage A533B(steel) 45 C cleavage LowCarbonSteel 50 C cleavage A515(steel) +20 C cleavage ASTM710GradeA +20 C ductile Literature does not announce the Qstress catalogue and Qstress value as functions of the external load, material properties or geometry of the specimen. The numerical analysis shown in Graba(2008) indicates that the Q parameter depends on material properties, specimen geometry and external load. In some papers,anengineermayfindjqgraphsforacertaingroupofmaterials.the best solution will be the catalogue of JQ graphs for materials characterised by various yield strengths, different workhardening exponents. Such a catalogue should take into consideration the influence of the external load, kind of the specimen(sen(b) specimen bending, CC(T) tension or SEN(T) tension) and its geometry. For SEN(B) specimens, such a catalogue was presented in Graba(2008), who presented Qstress values for specimens with predominance of bending for different materials and crack lengths. In the literature, there is no similar catalogue for specimens with predominance of tension. That is why,inthenextpartsofthepaper,valuesoftheqstresswillbedetermined for various elasticplastic materials for a centrally cracked plate in tension (CC(T)). The CC(T) specimen is the basic structural element which is used in the FITNET procedures(fitnet, 2006) to the modelling of real structures. Allresultswillbepresentedinagraphicalform theq=f(j)graphs.next, the numerical results will be approximated by closed form formulas. 3. Details of numerical analysis In the numerical analysis, the centrally cracked plate in tension(cc(t)) was used(fig. 3). Dimensions of the specimens satisfy the standard requirement whichissetupinfemcalculation L 2W,whereWisthewidthofthe specimen and L is the measuring length of the specimen. Computations were
7 The influence of material properties and crack length performed for a plane strain using small strain option. The relative crack lengthwas a/w={0.05,0.20,0.50,0.70}where aisthecracklength.the widthofspecimenswwasequalto40mm(forthiscase,themeasuringlength L 80mm).AllgeometricaldimensionsoftheCC(T)specimenarepresented intable2. Fig. 3. Centrally cracked plate in tension(cc(t)) Table 2. Geometrical dimensions of the CC(T) specimen used in numerical analysis width W [mm] measuring total relative crack crack length length length length 4W[mm] 2L[mm] a/w a[mm] The choice of the CC(T) specimen was intentional, because the CC(T) specimens are used in the FITNET procedures(fitnet, 2006) for modelling of real structural elements. Also in the FITNET procedures, the limit load and stress intensity factors for CC(T) specimens are presented. However in the EPRI procedures(kumar et al., 1981), the hybrid method for calculation of the Jintegral, crack opening displacement(cod) or crack tip opening displacement(ctod) are given. Also some laboratory tests in order to determine the critical values of the Jintegral may be done using the CC(T) specimen, see for example Sumpter and Forbes(1992).
8 30 M. Graba Computations were performed using ADINA SYSTEM 8.4 (ADINA, 2006a,b). Due to the symmetry, only a quarter of the specimen was modelled. The finite element mesh was filled with 9node plane strain elements. The size of the finite elements in the radial direction was decreasing towards the crack tip, while in the angular direction the size of each element was kept constant. Thecracktipregionwasmodelledusing36semicircles.Thefirstofthemwas 25timessmallerthanthelastone.Italsomeansthatthefirstfiniteelement behindthecracktipwassmaller2000timesthanthewidthofthespecimen. Thecracktipwasmodelledasaquarterofthearcwhoseradiuswasequalto r w =(12.5) 10 6 m.figure4presentsexemplaryfiniteelementmodelfor CC(T) specimen. Fig.4.(a)ThefiniteelementmodelforCC(T)specimenusedinthenumerical analysis(due to the symmetry, only a quarter of the specimen was modelled); (b)thecracktipmodelusedforthecc(t)specimen In the FEM simulation, the deformation theory of plasticity and the von Misses yield criterion were adopted. In the model, the stressstrain curve was approximated by the relation ε ε 0 = { σ/σ0 for σ σ 0 α(σ/σ 0 ) n for σ>σ 0 where α=1 (3.1) The tensile properties for materials which were used in the numerical analysis are presented below in Table 3. In the FEM analysis, calculations were done
9 The influence of material properties and crack length for sixteen materials, which differed by the yield stress and the work hardening exponent. Table 3. Mechanical properties of the materials used in numerical analysis (σ 0 yieldstress,e Young smoduluslν Poisson sratio,ε 0 straincorrespondingtheyieldstress,α constantinthepowerlawrelationship,nwork hardening exponent used in Eq.(3.1)) σ 0 [MPa] E[MPa] ν ε 0 =σ 0 /E α n The Jintegral was estimated using the virtual shift method. It uses the concept of virtual crack growth to compute virtual energy change(adina, 2006a,b). In the numerical analysis, 64 CC(T) specimens were used, which differed by the crack length(different a/w) and material properties(different ratios σ 0 /Eandvaluesofthepowerexponentn). 4. Numerical results analysis of JQ trajectories for CC(T) specimens The analysis of the results obtained by the finite element method showed that intherangeofdistancefromthecracktipj/σ 0 <r<6j/σ 0,theQstress decreases if the distance from the crack tip increases(fig. 5). If the external load increases, the Qstress decreases and the difference between the Qstress calculated in the following measurement points(distance r from the crack tip) increases(fig. 5). ForthesakeofthefactthattheQparameter,whichisusedinthefracture criterion,iscalculatedatadistanceequaltor=2j/σ 0 (whichwasproposed byo DowdandShih(1991,1992)),itisnecessarytocarryoutfullanalysisof the obtained results at this distance from the crack tip. Assessingtheinfluenceofthecracklengthonthe Qstressvalue,itis necessary to notice that if the crack length decreases, then the Qstress reachesagreaternegativevalueforthesamejintegrallevel seefig.6.for CC(T) specimens characterised by a short crack, the JQ curves reach faster the saturation level than for CC(T) specimens characterised by normative
10 32 M. Graba Fig. 5. The JQ family curves for CC(T) specimen calculated at six distances r forplanestrain(w=40mm,a/w=0.50,n=10,ν=0.3,e=206000mpa, σ 0 =1000MPa,ε 0 =σ 0 /E= );(a)wholeloadingspectrum,(b)magnified portion of the graph Fig.6.TheinfluenceofthecracklengthontheJQtrajectoriesforCC(T)specimen characterisedbyw=40mm,n=10,ν=0.3,e=206000mpa,σ 0 =1000MPa, ε 0 =σ 0 /E= (planestrainatthedistancefromthecracktipr=2J/σ 0 ) (a/w=0.50)andlong(a/w=0.70)cracks.itmaybenoticedthatforshort cracks, faster changes of the Qparameter are observed if the external load increases(see the graphs in Appendices). As shown in Fig. 7, if the yield stress increases, the Qparameter increases too, and it reflects for all CC(T) specimens with different crack lengths a/w.forsmalleryieldstresses,thejqtrajectoriesshapeuplower,andfaster changes of the Qparameter are observed if the external load is increases
11 The influence of material properties and crack length (Fig.7).ComparingtheJQtrajectoriesfordifferentvaluesofσ 0 /E,itisobserved that the biggest differences are characterised for materials with a small workhardening exponent(n = 3 for strongly workhardening materials) and the smallest for materials characterised by large workhardening exponents (n = 20 for weakly workhardening materials) see the graphs in Appendices. If the crack length increases, this difference somewhat increases too. For smaller yield stresses, the JQ curves for CC(T) specimens reach the saturation level for bigger external loads than the JQ curves for CC(T) specimens characterised by large yield stresses. Fig.7.TheinfluenceoftheyieldstressonJQ(a)andQ=f(log[J/(aσ 0 )])(b) trajectoriesforcc(t):w=40mm,a/w=0.50,n=10,ν=0.3,e=206000mpa (planestrainforthedistancefromthecracktipr=2j/σ 0 ) Figures8and9presentsomegraphsoftheJQtrajectorieswhichshowthe influenceoftheworkhardeningexponentnontheqstressvalueandjqcurves. If the yield stress decreases, the differences between the JQ trajectories characterised for materials described by different workhardening exponents are bigger. For CC(T) specimens, ambiguous behaviour of the JQ trajectories depending of the workhardening exponent is observed in comparison with SEN(B) specimens, which was presented in Graba(2008). In most cases(differentrelativecracklengthsa/w,differentyieldstresses(σ 0 /E )), if the workhardening exponent is smaller(strongly workhardening materials) than the Qstress value increases(fig. 9b). For small yield stresses ( σ / E ),iftheexternalloadincreases,thentheQstress value decreases if the workhardening exponent decreases(fig. 8a). For materialscharacterisedbytheyieldstressσ 0 /E= ,thedifferencebetween the JQ trajectories are small. Mutual intersecting and overlapping of the trajectories are observed too(fig. 9a).
12 34 M. Graba Fig.8.TheinfluenceoftheworkhardeningexponentonJQ(a)and Q=f(log[J/(aσ 0 )])(b)trajectoriesforcc(t):w=40mm,a/w=0.20,ν=0.3, E=206000MPa,σ 0 =315MPa,ε 0 =σ 0 /E= (planestrainforthedistance fromthecracktipr=2j/σ 0 ) Fig. 9. The influence of the workhardening exponent on JQ trajectories for CC(T):W=40mm,ν=0.3,E=206000MPaand(a)a/W=0.50,σ 0 =500MPa, ε 0 =σ 0 /E= ,(b)a/W=0.70,σ 0 =1000MPa,ε 0 =σ 0 /E= (plane strainforthedistancefromthecracktipr=2j/σ 0 ) 5. Approximation of the numerical results for CC(T) specimens All the obtained in the numerical analysis results were used to create a catalogue of the JQ trajectories for different specimens(characterised by different loading application, crack length) and different materials. The presented in the paper results are complementary with the directory presented in 2008 for SEN(B) specimens(graba, 2008). The current paper gives full numerical re
13 The influence of material properties and crack length sults for specimens with predominance of tension. The previous paper, which was mentioned above, gave numerical results and their approximation for specimens with predominance of bending. The presented numerical computations provided the JQ catalogue and universal formula(5.1) which allows one to calculate the Qstress for CC(T) specimens and take into consideration all the parameters influencing the value oftheqstress.allresultswerepresentedintheq=f(log[j/(aσ 0 )])graph forms(forexampleseefig.8bandfig.10). Fig.10.TheinfluenceoftheworkhardeningexponentonQ=f(log[J/(aσ 0 )]) trajectoriesforsen(b)specimen:w=40mm,ν=0.3,e=206000mpa, (a)a/w=0.50,σ 0 =500MPa,ε 0 =σ 0 /E= and(b)a/W=0.70, σ 0 =1000MPa,ε 0 =σ 0 /E= ;whichwereusedintheprocedureof approximation Next, all graphs were approximated by simple mathematical formulas taking the material properties, external load and geometry of the specimen into consideration. All the approximations were made for the results obtained at thedistancer=2j/σ 0.EachoftheobtainedtrajectoriesQ=f(log[J/(aσ 0 )]) was approximated by the third order polynomial in the form Q(J,a,σ 0 )=A+Blog J +C (log J ) 2+D ( log J ) 3 (5.1) aσ 0 aσ 0 aσ 0 wherethea,b,c,dcoefficientsdependontheworkhardeningexponentn, yieldstress σ 0 andcracklength a/w.therankofthefittingofformula (5.1)tonumericalresultsfortheworstcasewasequal R 2 =0.94forthe cracklengtha/w=0.05.forothercracklengthsa/w={0.20,0.50,0.70}, therankofthefittingofformula(5.1)satisfiedthecondition R Fordifferentworkhardeningexponentsn,yieldstressesσ 0 andratiosa/w,
14 36 M. Graba which were not included in the numerical analysis, the coefficients A, B, C and D may be evaluated using the linear or quadratic approximation. The results of numerical approximation using formula(5.1) for CC(T) specimens (allcoefficientsandtherankofthefitting)arepresentedintables47. Table 4. Coefficients of equation(5.1) for CC(T) specimen with the crack lengtha/w=0.05 n A B C D R 2 σ 0 =315MPa,σ 0 /E= σ 0 =1000MPa,σ 0 /E= σ 0 =500MPa,σ 0 /E= σ 0 =1500MPa,σ 0 /E= Table 5. Coefficients of equation(5.1) for CC(T) specimen with the crack lengtha/w=0.20 n A B C D R 2 σ 0 =315MPa,σ 0 /E=
15 The influence of material properties and crack length σ 0 =1000MPa,σ 0 /E= σ 0 =500MPa,σ 0 /E= σ 0 =1500MPa,σ 0 /E= Table 6. Coefficients of equation(5.1) for CC(T) specimen with the crack lengtha/w=0.50 n A B C D R 2 σ 0 =315MPa,σ 0 /E= σ 0 =1000MPa,σ 0 /E= σ 0 =500MPa,σ 0 /E=
16 38 M. Graba σ 0 =1500MPa,σ 0 /E= Table 7. Coefficients of equation(5.1) for CC(T) specimen with the crack lengtha/w=0.70 n A B C D R 2 σ 0 =315MPa,σ 0 /E= σ 0 =1000MPa,σ 0 /E= σ 0 =500MPa,σ 0 /E= σ 0 =1500MPa,σ 0 /E= Figure 11 presents the comparison of the numerical results and their approximation for JQ trajectories for several cases of the CC(T) specimens. Appendices AD attached to the paper present in a graphical form(figs ) all numerical results obtained for CC(T) specimens in plain strain. All results are presented using the JQ trajectories for each analyzed case.
17 The influence of material properties and crack length Fig. 11. Comparison of the numerical results and their approximation for JQ trajectoriesforcc(t)specimens:w=40mm,a/w=0.50,e=206000mpa, ν=0.3and(a)σ 0 {315,500}MPa,n {5,10},(b)σ 0 {1000,1500}MPa, n {10,20} 6. Conclusions In the paper, values of the Qstress were determined for various elasticplastic materials for centrally cracked plate in tension(cc(t)). The influence of the yield strength, the workhardening exponent and the crack length on the Q parameter was tested. The numerical results were approximated by closed form formulas. In summary, it may be concluded that the Qstress depends on geometry and the external load. Different values of the Qstress are obtained for a centrally cracked plane in tension(cc(t)) and different for the SEN(B) specimen, which was characterised by the same material properties(see Appendices of this paper and Appendices in Graba(2008)). The Qparameter is a function of the material properties; its value depends on the workhardening exponentnandtheyieldstressσ 0.Ifthecracklengthdecreases,thenQstress reaches greater negative value for the same external load. The presented in the paper catalogue of the Qstress values and JQ trajectories for specimens with predominance of tension(cc(t) specimens) is complementary with the numerical solution presented in Graba(2008), which gave JQ trajectories for specimens with predominance of bending(sen(b) specimens)). Both papers may be quite useful for solving engineering problems in which the fracture toughness or stress distribution near the crack tip must be quite fast estimated.
18 40 M. Graba Appendix A. Numerical results for CC(T) specimen in plane strain withthecracklengtha/w=0.05(distancefromthecracktip r=2j/σ 0 ) Fig. 12. The influence of the yield stress on JQ trajectories for CC(T) specimens withthecracklengtha/w=0.05fordifferentpowerexponentsinro relationship:(a)n=3,(b)n=5,(c)n=10,(d)n=20(w=40mm,ν=0.3, E=206000MPa)
19 The influence of material properties and crack length Appendix B. Numerical results for CC(T) specimen in plane strain withthecracklengtha/w=0.20(distancefromthecracktip r=2j/σ 0 ) Fig. 13. The influence of the yield stress on JQ trajectories for CC(T) specimens withthecracklengtha/w=0.20fordifferentpowerexponentsinro relationship:(a)n=3,(b)n=5,(c)n=10,(d)n=20(w=40mm,ν=0.3, E=206000MPa)
20 42 M. Graba Appendix C. Numerical results for CC(T) specimen in plane strain withthecracklengtha/w=0.50(distancefromthecracktip r=2.j/σ 0 ) Fig. 14. The influence of the yield stress on JQ trajectories for CC(T) specimens withthecracklengtha/w=0.50fordifferentpowerexponentsinro relationship:(a)n=3,(b)n=5,(c)n=10,(d)n=20(w=40mm,ν=0.3, E=206000MPa)
21 The influence of material properties and crack length Appendix D. Numerical results for CC(T) specimen in plane strainwiththecracklengtha/w=0.70(distancefromthecrack tipr=2j/σ 0 ) Fig. 15. The influence of the yield stress on JQ trajectories for CC(T) specimens withthecracklengtha/w=0.70fordifferentpowerexponentsinro relationship:(a)n=3,(b)n=5,(c)n=10,(d)n=20(w=40mm,ν=0.3, E=206000MPa) Acknowledgements The support of Kielce University of Technology, Faculty of Mechatronics and Machine Design through grant No. 1.22/8.57 is acknowledged by the author of the paper.
22 44 M. Graba References 1. ADINA 2006a, ADINA 8.4.1: User Interface Command Reference Manual Volume I: ADINA Solids& Structures Model Definition, Report ARD 062, ADINA R&D, Inc. 2. ADINA 2006b, ADINA 8.4.1: Theory and Modeling Guide Volume I: ADINA, Report ARD 067, ADINA R&D, Inc. 3. Ainsworth R.A., O Dowd N.P., 1994, A framework of including constraint effects in the failure assessment diagram approach for fracture assessment, ASME Pressure Vessels and Piping Conference, ASME, PVPVol 287/MD Vol47 4. FITNET, 2006, FITNET Report,(European Fitnessforservice Network), Edited by M. Kocak, S. Webster, J.J. Janosch, R.A. Ainsworth, R. Koers, Contract No. G1RTCT GałkiewiczJ.,GrabaM.,2006,Algorithmfordeterminationof σ ij (n,θ), ε ij (n,θ),ũ i (n,θ),d n (n),andi n (n)functionsinhutchinsonricerosengrensolution and its 3D generalization, Journal of Theoretical and Applied Mechanics, 44,1, Graba M., 2008, The influence of material properties on the Qstress value near the crack tip for elasticplastic materials, Journal of Theoretical and Applied Mechanics, 46, 2, HutchinsonJ.W.,1968,Singularbehaviourattheendofatensilecrackina hardening material, Journal of the Mechanics and Physics of Solids, 16, Kumar V., German M.D., Shih C.F., 1981, An engineering approach for elasticplastic fracture analysis, EPRI Report NP1931, Electric Power Research Institute, Palo Alto, CA 9. Li Y., Wang Z., 1985, Highorder asymptotic field of tensile planestrain nonlinear crack problems, Scientia Sinica(Series A), XXIX, 9, NeimitzA.,DziobaI.,MolasyR.,GrabaM.,2004,Wpływwięzównaodporność na pękanie materiałów kruchych, Materiały XX Sympozjum Zmęczenia i Mechaniki Pękania, BydgoszczPieczyska, Neimitz A., Graba M., Gałkiewicz J., 2007, An alternative formulation of the RitchieKnottRice local fracture criterion, Engineering Fracture Mechanics, 74, O Dowd N.P., 1995, Applications of two parameter approaches in elasticplastic fracture mechanics, Engineering Fracture Mechanics, 52, 3, O Dowd N.P., Shih C.F., 1991, Family of cracktip fields characterized by atriaxialityparameter I.Structureoffields,J.Mech.Phys.Solids,39,8,
HOW RESIDUAL STRESSES AFFECT PREDICTION OF BRITTLE FRACTURE
HOW RESIDUAL STRESSES AFFECT PREDICTION OF BRITTLE FRACTURE Michael R. Hill Mechanical and Aeronautical Engineering Department University of California, Davis mrhill@ucdavis.edu Tina L. Panontin Systems
More informationNOTCHES AND THEIR EFFECTS. Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 1
NOTCHES AND THEIR EFFECTS Ali Fatemi  University of Toledo All Rights Reserved Chapter 7 Notches and Their Effects 1 CHAPTER OUTLINE Background Stress/Strain Concentrations SN Approach for Notched Members
More informationTensile fracture analysis of blunt notched PMMA specimens by means of the Strain Energy Density
Engineering Solid Mechanics 3 (2015) 3542 Contents lists available at GrowingScience Engineering Solid Mechanics homepage: www.growingscience.com/esm Tensile fracture analysis of blunt notched PMMA specimens
More informationB. INTRODUCTION TO ASSESSMENT PROCEDURES FOR CRACKED COMPONENTS
B. INTRODUCTION TO ASSESSMENT PROCEDURES FOR CRACKED COMPONENTS 40 INTRODUCTION HOW ARE INTEGRITY, SECURITY OR CRITICAL CONDITIONS ANALYSED IN A CRACKED STRUCTURE? FRACTURE MECHANICS Critical conditions
More informationStructural Integrity Analysis
Structural Integrity Analysis 1. STRESS CONCENTRATION Igor Kokcharov 1.1 STRESSES AND CONCENTRATORS 1.1.1 Stress An applied external force F causes inner forces in the carrying structure. Inner forces
More informationYield Criteria for Ductile Materials and Fracture Mechanics of Brittle Materials. τ xy 2σ y. σ x 3. τ yz 2σ z 3. ) 2 + ( σ 3. σ 3
Yield Criteria for Ductile Materials and Fracture Mechanics of Brittle Materials Brittle materials are materials that display Hookean behavior (linear relationship between stress and strain) and which
More information2. FRACTURE MECHANICS
2. FRACTURE MECHANICS Igor Kokcharov 2.1 DEFECTS Structural materials have inner defects such as cracks, which are extreme stress concentrators. There are technological defects shown in diagrams A and
More informationCOMPUTATIONAL ENGINEERING OF FINITE ELEMENT MODELLING FOR AUTOMOTIVE APPLICATION USING ABAQUS
International Journal of Advanced Research in Engineering and Technology (IJARET) Volume 7, Issue 2, MarchApril 2016, pp. 30 52, Article ID: IJARET_07_02_004 Available online at http://www.iaeme.com/ijaret/issues.asp?jtype=ijaret&vtype=7&itype=2
More informationObjective To conduct Charpy Vnotch impact test and determine the ductilebrittle transition temperature of steels.
IMPACT TESTING Objective To conduct Charpy Vnotch impact test and determine the ductilebrittle transition temperature of steels. Equipment Coolants Standard Charpy VNotched Test specimens Impact tester
More informationBurst Pressure Prediction of Pressure Vessel using FEA
Burst Pressure Prediction of Pressure Vessel using FEA Nidhi Dwivedi, Research Scholar (G.E.C, Jabalpur, M.P), Veerendra Kumar Principal (G.E.C, Jabalpur, M.P) Abstract The main objective of this paper
More informationFITNET Fitnessforservice Fracture Module SOFTWARE
Nenad Gubeljak Associate Professor University of Maribor Faculty of Mechanical Engineering Mustafa Koçak European FitnessforService Network FITNET coordinator GKSS Research Centre Institute for Materials
More informationMETU DEPARTMENT OF METALLURGICAL AND MATERIALS ENGINEERING
METU DEPARTMENT OF METALLURGICAL AND MATERIALS ENGINEERING Met E 206 MATERIALS LABORATORY EXPERIMENT 1 Prof. Dr. Rıza GÜRBÜZ Res. Assist. Gül ÇEVİK (Room: B306) INTRODUCTION TENSION TEST Mechanical testing
More informationStress Strain Relationships
Stress Strain Relationships Tensile Testing One basic ingredient in the study of the mechanics of deformable bodies is the resistive properties of materials. These properties relate the stresses to the
More informationANALYTICAL AND EXPERIMENTAL EVALUATION OF SPRING BACK EFFECTS IN A TYPICAL COLD ROLLED SHEET
International Journal of Mechanical Engineering and Technology (IJMET) Volume 7, Issue 1, JanFeb 2016, pp. 119130, Article ID: IJMET_07_01_013 Available online at http://www.iaeme.com/ijmet/issues.asp?jtype=ijmet&vtype=7&itype=1
More informationEstimation of the crack propagation direction in a mixedmode geometry via multiparameter fracture criteria
Focussed on characterization of crack tip fields Estimation of the crack propagation direction in a mixedmode geometry via multiparameter fracture criteria L. Malíková, V. Veselý Brno University of Technology,
More informationELASTOPLASTIC ANALYSIS OF A HEAVY DUTY PRESS USING F.E.M AND NEUBER S APPROXIMATION METHODS
International Journal of Mechanical Engineering and Technology (IJMET) Volume 6, Issue 11, Nov 2015, pp. 5056, Article ID: IJMET_06_11_006 Available online at http://www.iaeme.com/ijmet/issues.asp?jtype=ijmet&vtype=6&itype=11
More informationEXPERIMENTAL AND NUMERICAL ANALYSIS OF THE COLLAR PRODUCTION ON THE PIERCED FLAT SHEET METAL USING LASER FORMING PROCESS
JOURNAL OF CURRENT RESEARCH IN SCIENCE (ISSN 23225009) CODEN (USA): JCRSDJ 2014, Vol. 2, No. 2, pp:277284 Available at www.jcrs010.com ORIGINAL ARTICLE EXPERIMENTAL AND NUMERICAL ANALYSIS OF THE COLLAR
More informationG1RTCT200105071 D. EXAMPLES F. GUTIÉRREZSOLANA S. CICERO J.A. ALVAREZ R. LACALLE W P 6: TRAINING & EDUCATION
D. EXAMPLES 316 WORKED EXAMPLE I Infinite Plate under fatigue Introduction and Objectives Data Analysis 317 INTRODUCTION AND OBJECTIVES One structural component of big dimensions is subjected to variable
More informationSTRAINLIFE (e N) APPROACH
CYCLIC DEFORMATION & STRAINLIFE (e N) APPROACH MONOTONIC TENSION TEST AND STRESSSTRAIN BEHAVIOR STRAINCONTROLLED TEST METHODS CYCLIC DEFORMATION AND STRESSSTRAIN BEHAVIOR STRAINBASED APPROACH TO
More informationFatigue Testing. Objectives
Laboratory 8 Fatigue Testing Objectives Students are required to understand principle of fatigue testing as well as practice how to operate the fatigue testing machine in a reverse loading manner. Students
More informationVersion default Titre : SSNP161 Essais biaxiaux de Kupfer Date : 10/10/2012 Page : 1/8 Responsable : François HAMON Clé : V6.03.161 Révision : 9783
Titre : SSNP161 Essais biaxiaux de Kupfer Date : 10/10/2012 Page : 1/8 SSNP161 Biaxial tests of Summarized Kupfer: Kupfer [1] was interested to characterize the performances of the concrete under biaxial
More informationTorsion Tests. Subjects of interest
Chapter 10 Torsion Tests Subjects of interest Introduction/Objectives Mechanical properties in torsion Torsional stresses for large plastic strains Type of torsion failures Torsion test vs.tension test
More informationCH 6: Fatigue Failure Resulting from Variable Loading
CH 6: Fatigue Failure Resulting from Variable Loading Some machine elements are subjected to static loads and for such elements static failure theories are used to predict failure (yielding or fracture).
More informationTechnical Report Example (1) Chartered (CEng) Membership
Technical Report Example (1) Chartered (CEng) Membership A TECHNICAL REPORT IN SUPPORT OF APPLICATION FOR CHARTERED MEMBERSHIP OF IGEM DESIGN OF 600 (103 BAR) 820MM SELF SEALING REPAIR CLAMP AND VERIFICATION
More informationNumerical Analysis of Independent Wire Strand Core (IWSC) Wire Rope
Numerical Analysis of Independent Wire Strand Core (IWSC) Wire Rope Rakesh Sidharthan 1 Gnanavel B K 2 Assistant professor Mechanical, Department Professor, Mechanical Department, Gojan engineering college,
More informationTechnology of EHIS (stamping) applied to the automotive parts production
Laboratory of Applied Mathematics and Mechanics Technology of EHIS (stamping) applied to the automotive parts production Churilova Maria, SaintPetersburg State Polytechnical University Department of Applied
More informationLap Fillet Weld Calculations and FEA Techniques
Lap Fillet Weld Calculations and FEA Techniques By: MS.ME Ahmad A. Abbas Sr. Analysis Engineer Ahmad.Abbas@AdvancedCAE.com www.advancedcae.com Sunday, July 11, 2010 Advanced CAE All contents Copyright
More informationIMPELLER FATIGUE ASSESSMENT USING AN SN APPROACH
ENGINEERING PAPER 524408 IMPELLER FATIGUE ASSESSMENT USING AN SN APPROACH Samuel Orr Engineering Analysis Manager Howden Technology AMCA International Engineering Conference Las Vegas, NV, USA 2 4 March
More informationME111 Lecture 16 1. ME111 Instructor: Peter Pinsky Class #16 November 1, 2000
Toda s Topics ME111 Instructor: Peter Pinsk Class #16 November 1, 2000 Introduction to linear elastic fracture mechanics (LEFM). Problem 3 A centercracked plate of AII 1144 steel ( C = 115MPa m ) has
More informationLABORATORY EXPERIMENTS TESTING OF MATERIALS
LABORATORY EXPERIMENTS TESTING OF MATERIALS 1. TENSION TEST: INTRODUCTION & THEORY The tension test is the most commonly used method to evaluate the mechanical properties of metals. Its main objective
More informationC. PROCEDURE APPLICATION (FITNET)
C. PROCEDURE APPLICATION () 495 INTRODUCTION ASSESSMENT OF SCC ASSESSMENT OF CORROSION FATIGUE STRESS CORROSION AND CORROSION FATIGUE ANALYSIS ASSESSMENT OF LOCAL THINNED AREAS 496 INTRODUCTION INTRODUCTION
More informationFatigue Analysis and Optimization of Flexible Printed Circuits
Fatigue Analysis and Optimization of Flexible Printed Circuits Alexander Ptchelintsev Nokia Research Center P.O. Box 407, FI00045 NOKIA GROUP, Finland Email: alexander.ptchelintsev@nokia.com Abstract:
More informationObjectives. Experimentally determine the yield strength, tensile strength, and modules of elasticity and ductility of given materials.
Lab 3 Tension Test Objectives Concepts Background Experimental Procedure Report Requirements Discussion Objectives Experimentally determine the yield strength, tensile strength, and modules of elasticity
More informationShort and Large Crack, MixedMode FatigueCrack Growth Thresholds in Ti6Al4V 1
Short and Large Crack, MixedMode FatigueCrack Growth Thresholds in Ti6Al4V 1 Mr. R. K. Nalla, Dr. J. P. Campbell and Professor R. O. Ritchie 2 Department of Materials Science and Engineering University
More informationChapter Outline. Mechanical Properties of Metals How do metals respond to external loads?
Mechanical Properties of Metals How do metals respond to external loads? Stress and Strain Tension Compression Shear Torsion Elastic deformation Plastic Deformation Yield Strength Tensile Strength Ductility
More informationDeflection Calculation of RC Beams: Finite Element Software Versus Design Code Methods
Deflection Calculation of RC Beams: Finite Element Software Versus Design Code Methods G. Kaklauskas, Vilnius Gediminas Technical University, 1223 Vilnius, Lithuania (gintaris.kaklauskas@st.vtu.lt) V.
More informationLecture 12: Fundamental Concepts in Structural Plasticity
Lecture 12: Fundamental Concepts in Structural Plasticity Plastic properties of the material were already introduced briefly earlier in the present notes. The critical slenderness ratio of column is controlled
More informationCADBASED DESIGN PROCESS FOR FATIGUE ANALYSIS, RELIABILITY ANALYSIS, AND DESIGN OPTIMIZATION
CADBASED DESIGN PROCESS FOR FATIGUE ANALYSIS, RELIABILITY ANALYSIS, AND DESIGN OPTIMIZATION K.K. Choi, V. Ogarevic, J. Tang, and Y.H. Park Center for ComputerAided Design College of Engineering The
More informationFatigue Performance Evaluation of Forged Steel versus Ductile Cast Iron Crankshaft: A Comparative Study (EXECUTIVE SUMMARY)
Fatigue Performance Evaluation of Forged Steel versus Ductile Cast Iron Crankshaft: A Comparative Study (EXECUTIVE SUMMARY) Ali Fatemi, Jonathan Williams and Farzin Montazersadgh Professor and Graduate
More informationTensile Testing Laboratory
Tensile Testing Laboratory By Stephan Favilla 0723668 ME 354 AC Date of Lab Report Submission: February 11 th 2010 Date of Lab Exercise: January 28 th 2010 1 Executive Summary Tensile tests are fundamental
More informationSTATIC AND DYNAMIC ANALYSIS OF CENTER CRACKED FINITE PLATE SUBJECTED TO UNIFORM TENSILE STRESS USING FINITE ELEMENT METHOD
INTERNATIONAL JOURNAL OF MECHANICAL ENGINEERING AND TECHNOLOGY (IJMET) International Journal of Mechanical Engineering and Technology (IJMET), ISSN 0976 6340(Print), ISSN 0976 6340 (Print) ISSN 0976 6359
More informationInteraction of Hydrogen and Deformation in 316L Stainless Steel
Proceedings of the SEM Annual Conference June 14, 2009 Albuquerque New Mexico USA 2009 Society for Experimental Mechanics Inc. Interaction of Hydrogen and Deformation in 316L Stainless Steel Bonnie R.
More informationBack to Elements  Tetrahedra vs. Hexahedra
Back to Elements  Tetrahedra vs. Hexahedra Erke Wang, Thomas Nelson, Rainer Rauch CADFEM GmbH, Munich, Germany Abstract This paper presents some analytical results and some test results for different
More informationMASTER DEGREE PROJECT
MASTER DEGREE PROJECT Finite Element Analysis of a Washing Machine Cylinder Thesis in Applied Mechanics one year Master Degree Program Performed : Spring term, 2010 Level Author Supervisor s Examiner :
More informationFinite Element Analysis on Burst Pressure of Defective Steel Pipes
Finite Element Analysis on Burst Pressure of Defective Steel Pipes N. A. Alang 1, N. A. Razak 2, K.A.Safie 3, and A. Sulaiman 4 Faculty of Mechanical Engineering, Universiti Malaysia Pahang, 266, Pekan,
More informationINJECTION MOLDING COOLING TIME REDUCTION AND THERMAL STRESS ANALYSIS
INJECTION MOLDING COOLING TIME REDUCTION AND THERMAL STRESS ANALYSIS Tom Kimerling University of Massachusetts, Amherst MIE 605 Finite Element Analysis Spring 2002 ABSTRACT A FEA transient thermal structural
More informationPunching shear behavior of steelconcrete composite decks with different shear connectors
Punching shear behavior of steelconcrete composite decks with different shear connectors *XiaoQing Xu 1) and YuQing Liu 2) 1), 2) Department of Bridge Engineering, Tongji University, Shanghai 200092,
More informationFEM analysis of the forming process of automotive suspension springs
FEM analysis of the forming process of automotive suspension springs Berti G. and Monti M. University of Padua, DTG, Stradella San Nicola 3, I36100 Vicenza (Italy) guido.berti@unipd.it, manuel.monti@unipd.it.
More informationNumerical Analysis of Cohesive Crack Growth Using Extended Finite Element Method (XFEM)
Ecole Centrale de Nantes (ECN) Institut de Recherche en Génie Civil et Méchanique (GeM) The International Center for Numerical Methods in Engineering (CIMNE) Master of Science Thesis Numerical Analysis
More informationESCUELA TÉCNICA SUPERIOR DE INGENIEROS INDUSTRIALES Y DE TELECOMUNICACIÓN
ESCUELA TÉCNICA SUPERIOR DE INGENIEROS INDUSTRIALES Y DE TELECOMUNICACIÓN Titulación: INGENIERO INDUSTRIAL Título del proyecto: MODELING CRACKS WITH ABAQUS Pablo Sanchis Gurpide Pamplona, 22 de Julio del
More informationTensile Testing of Steel
C 265 Lab No. 2: Tensile Testing of Steel See web for typical report format including: TITL PAG, ABSTRACT, TABL OF CONTNTS, LIST OF TABL, LIST OF FIGURS 1.0  INTRODUCTION See General Lab Report Format
More informationME 612 Metal Forming and Theory of Plasticity. 3. Work Hardening Models
Metal Forming and Theory of Plasticity Yrd.Doç. e mail: azsenalp@gyte.edu.tr Makine Mühendisliği Bölümü Gebze Yüksek Teknoloji Enstitüsü In this section work hardening models that are applicable to different
More informationdifferent levels, also called repeated, alternating, or fluctuating stresses.
Fatigue and Dynamic Loading 1 Fti Fatigue fil failure: 2 Static ti conditions : loads are applied gradually, to give sufficient i time for the strain to fully develop. Variable conditions : stresses vary
More informationFigure 1: Typical SN Curves
StressLife Diagram (SN Diagram) The basis of the StressLife method is the Wohler SN diagram, shown schematically for two materials in Figure 1. The SN diagram plots nominal stress amplitude S versus
More informationDescription of mechanical properties
ArcelorMittal Europe Flat Products Description of mechanical properties Introduction Mechanical properties are governed by the basic concepts of elasticity, plasticity and toughness. Elasticity is the
More information3. Test Methods for Evaluation of ESCR of Plastics
3. Test Methods for Evaluation of ESCR of Plastics A common laboratory request for ESCprone polymers is to check ESCR performance for quality control, competitive product evaluations, and research and
More informationTorsion Testing. Objectives
Laboratory 4 Torsion Testing Objectives Students are required to understand the principles of torsion testing, practice their testing skills and interpreting the experimental results of the provided materials
More informationPOLITECNICO DI TORINO. Engineering Faculty Master s Degree in Aerospace Engineering. Final Thesis
POLITECNICO DI TORINO Engineering Faculty Master s Degree in Aerospace Engineering Final Thesis DETECTION AND ANALYSIS OF BARELY VISIBLE IMPACT DAMAGE AND ITS PROGRESSION ON A COMPOSITE OVERWRAPPED PRESSURE
More informationσ y ( ε f, σ f ) ( ε f
Typical stressstrain curves for mild steel and aluminum alloy from tensile tests L L( 1 + ε) A =  A u u 0 1 E l mild steel fracture u ( ε f, f ) ( ε f, f ) ε 0 ε 0.2 = 0.002 aluminum alloy fracture
More informationMagnetic / Gravity Loading Analysis
Magnetic / Gravity Loading Analysis 2 ELEMENTS JUL 7 2006 ELEMENTS MAT NUM 2:5:0 MAT NUM POR Design JUL 7 2006 2:5:0 L2 L L q Assumed Location of Gap Encoder(s) ELEMENTS MAT NUM JUL 7 2006 2:5:0 Materials:
More informationNew Unified Fracture Toughness Estimation Scheme for Structural Integrity Assessment
ew Unified Fracture Toughness Estimation Scheme for Structural Integrity Assessment Kim Wallin, Research Professor Technical Research Centre of Finland Espoo, Finland Adam Bannister, Manager, Research
More informationMETHODS FOR ACHIEVEMENT UNIFORM STRESSES DISTRIBUTION UNDER THE FOUNDATION
International Journal of Civil Engineering and Technology (IJCIET) Volume 7, Issue 2, MarchApril 2016, pp. 4566, Article ID: IJCIET_07_02_004 Available online at http://www.iaeme.com/ijciet/issues.asp?jtype=ijciet&vtype=7&itype=2
More informationMaterial Challenges in Arctic Applications
1 Material Challenges in Arctic Applications  The KMB (Petromaks) project "Arctic Materials"  Akselsen OM, Østby E, Olafsen K, Stokke R SINTEF Materials and Chemistry 2 Outline Background Objectives
More informationDamage due to fatigue occurs when loading is markedly varying in time. R decreases with time S T. MSÚ F max
5. Fatigue of steel structures Fatigue loading, Wöhler s approach and fracture mechanics, fatigue strength, influence of notches, damage accumulation, Eurocode approach. Damage due to fatigue occurs when
More informationAC 20082887: MATERIAL SELECTION FOR A PRESSURE VESSEL
AC 20082887: MATERIAL SELECTION FOR A PRESSURE VESSEL Somnath Chattopadhyay, Pennsylvania State University American Society for Engineering Education, 2008 Page 13.869.1 Material Selection for a Pressure
More informationESTIMATION OF UNDRAINED SETTLEMENT OF SHALLOW FOUNDATIONS ON LONDON CLAY
International Conference on Structural and Foundation Failures August 24, 2004, Singapore ESTIMATION OF UNDRAINED SETTLEMENT OF SHALLOW FOUNDATIONS ON LONDON CLAY A. S. Osman, H.C. Yeow and M.D. Bolton
More informationEVALUATION OF SEISMIC RESPONSE  FACULTY OF LAND RECLAMATION AND ENVIRONMENTAL ENGINEERING BUCHAREST
EVALUATION OF SEISMIC RESPONSE  FACULTY OF LAND RECLAMATION AND ENVIRONMENTAL ENGINEERING BUCHAREST Abstract Camelia SLAVE University of Agronomic Sciences and Veterinary Medicine of Bucharest, 59 Marasti
More informationMechanical Properties of Metals Mechanical Properties refers to the behavior of material when external forces are applied
Mechanical Properties of Metals Mechanical Properties refers to the behavior of material when external forces are applied Stress and strain fracture or engineering point of view: allows to predict the
More informationPragmatic multiscale and multiphysics analysis of Charles Bridge in Prague
Pragmatic multiscale and multiphysics analysis of Charles Bridge in Prague Jiří Šejnoha 1,2 Michal Šejnoha 1,2 Jan Zeman 1 Jan Novák 1,2 with Zdeněk Janda, Jiří Maděra, Jan Vorel and Jan Sýkora 1 Department
More informationPRELIMINARY ANALYSIS OF INELASTIC BUCKLING OF THE HEAT EXCHANGER
JOURNAL OF THEORETICAL AND APPLIED MECHANICS 46, 2, pp. 305313, Warsaw 2008 PRELIMINARY ANALYSIS OF INELASTIC BUCKLING OF THE HEAT EXCHANGER Agnieszka Chudzik Technical University of Lodz, Division of
More informationSolid Mechanics. Stress. What you ll learn: Motivation
Solid Mechanics Stress What you ll learn: What is stress? Why stress is important? What are normal and shear stresses? What is strain? Hooke s law (relationship between stress and strain) Stress strain
More informationTR1029. Technical Report. Damage tolerance analysis of canister inserts for spent nuclear fuel in the case of an earthquake induced rock shear load
Technical Report TR129 Damage tolerance analysis of canister inserts for spent nuclear fuel in the case of an earthquake induced rock shear load Peter Dillström, Tobias Bolinder Inspecta Technology AB
More informationMultiaxial Fatigue. Professor Darrell Socie. 20082014 Darrell Socie, All Rights Reserved
Multiaxial Fatigue Professor Darrell Socie 20082014 Darrell Socie, All Rights Reserved Outline Stresses around holes Crack Nucleation Crack Growth MultiaxialFatigue 20082014 Darrell Socie, All Rights
More informationDesign and Analysis of Vapour Absorbing Machine
Vol. 3, Issue. 4, Jul  Aug. 2013 pp21612165 ISSN: 22496645 Design and Analysis of Vapour Absorbing Machine Prashant Tile 1, S. S.Barve 2 12 Department 100 of Mechanical Engineering, VJTI, Mumbai, India
More informationAn Overview of the Finite Element Analysis
CHAPTER 1 An Overview of the Finite Element Analysis 1.1 Introduction Finite element analysis (FEA) involves solution of engineering problems using computers. Engineering structures that have complex geometry
More informationFatigue Resistance of High Strength Bolts with Large Diameters
1 Fatigue Resistance of High Strength Bolts with Large Diameters Prof. Peter Schaumann; Dipl.Ing. Frithjof Marten Leibniz Universitaet Hannover Institute for Steel Construction Hannover, Germany schaumann@stahl.unihannover.de;
More informationMODELING THE EFFECT OF TEMPERATURE AND FREQUENCY ON BITUMENCOATED HELICAL CABLE ELEMENTS
MODELING THE EFFECT OF TEMPERATURE AND FREQUENCY ON BITUMENCOATED HELICAL CABLE ELEMENTS Bjørn Konradsen 1 Technological Analyses Centre, Hybrid Underwater Cables, Nexans Norway Steinar V. Ouren Material
More informationSolved with COMSOL Multiphysics 4.3
Vibrating String Introduction In the following example you compute the natural frequencies of a pretensioned string using the 2D Truss interface. This is an example of stress stiffening ; in fact the
More informationDEVELOPMENT OF A NEW TEST FOR DETERMINATION OF TENSILE STRENGTH OF CONCRETE BLOCKS
1 th Canadian Masonry Symposium Vancouver, British Columbia, June 5, 013 DEVELOPMENT OF A NEW TEST FOR DETERMINATION OF TENSILE STRENGTH OF CONCRETE BLOCKS Vladimir G. Haach 1, Graça Vasconcelos and Paulo
More informationABAQUS for CATIA V5 Tutorials
ABAQUS for CATIA V5 Tutorials AFC V2 Nader G. Zamani University of Windsor Shuvra Das University of Detroit Mercy SDC PUBLICATIONS Schroff Development Corporation www.schroff.com www.schroffeurope.com
More informationEstimation of shear force for blind shear ram blowout preventers
Estimation of shear force for blind shear ram blowout preventers Abdulkadir Tekin *, Changhyok Choi, Taylan Altan, Hamit Adin Online Publication Date: 17 Feb 2015 URL: http://www.jresm.org/archive/resm2014.02st1225.html
More informationANALYSIS OF A LAP JOINT FRICTION CONNECTION USING HIGH STRENGTH BOLTS
Nordic Steel Construction Conference 212 Hotel Bristol, Oslo, Norway 57 September 212 ANALYSIS OF A LAP JOINT FRICTION CONNECTION USING HIGH STRENGTH BOLTS Marouene Limam a, Christine Heistermann a and
More informationMechanical Properties
Mechanical Properties Hardness Hardness can be defined as resistance to deformation or indentation or resistance to scratch. Hardness Indentation Scratch Rebound Indentation hardness is of particular interest
More informationNumerical modelling of shear connection between concrete slab and sheeting deck
7th fib International PhD Symposium in Civil Engineering 2008 September 1013, Universität Stuttgart, Germany Numerical modelling of shear connection between concrete slab and sheeting deck Noémi Seres
More informationNonlinear Models of Reinforced and Posttensioned Concrete Beams
111 Nonlinear Models of Reinforced and Posttensioned Concrete Beams ABSTRACT P. Fanning Lecturer, Department of Civil Engineering, University College Dublin Earlsfort Terrace, Dublin 2, Ireland. Email:
More information9. TIME DEPENDENT BEHAVIOUR: CYCLIC FATIGUE
9. TIME DEPENDENT BEHAVIOUR: CYCLIC FATIGUE A machine part or structure will, if improperly designed and subjected to a repeated reversal or removal of an applied load, fail at a stress much lower than
More informationCOMPARISON OF STRESS BETWEEN WINKLERBACH THEORY AND ANSYS FINITE ELEMENT METHOD FOR CRANE HOOK WITH A TRAPEZOIDAL CROSSSECTION
COMPARISON OF STRESS BETWEEN WINKLERBACH THEORY AND ANSYS FINITE ELEMENT METHOD FOR CRANE HOOK WITH A TRAPEZOIDAL CROSSSECTION Yogesh Tripathi 1, U.K Joshi 2 1 Postgraduate Student, 2 Associate Professor,
More informationLong term performance of polymers
1.0 Introduction Long term performance of polymers Polymer materials exhibit time dependent behavior. The stress and strain induced when a load is applied are a function of time. In the most general form
More informationModelling of Contact Problems of Rough Surfaces
Modelling of Contact Problems of Rough Surfaces N. Schwarzer, Saxonian Institute of Surface Mechanics, Am Lauchberg 2, 04838 Eilenburg, Germany, Tel. ++49 (0) 3423 656639 or 58, Fax. ++49 (0) 3423 656666,
More information2.75 6.525 Problem Set 1 Solutions to ME problems Fall 2013
2.75 6.525 Problem Set 1 Solutions to ME problems Fall 2013 2. Pinned Joint problem Jacob Bayless a) Draw a freebody diagram for the pin. How is it loaded? Does the loading depend on whether the pin is
More informationFracture and strain rate behavior of airplane fuselage materials under blast loading
EPJ Web of Conferences 6, 6 42017 (2010) DOI:10.1051/epjconf/20100642017 Owned by the authors, published by EDP Sciences, 2010 Fracture and strain rate behavior of airplane fuselage materials under blast
More informationThe Material Properties of Cement Paste with Fly Ash Exposed to High Temperatures
The Material Properties of Cement Paste with Fly Ash Exposed to High s PAVEL PADEVĚT, ROMANA LOVICHOVÁ Department of Mechanics Czech Technical University in Prague Thákurova 7, 166 29, Prague 6 CZECH REPUBLIC
More informationUniaxial Tension and Compression Testing of Materials. Nikita Khlystov Daniel Lizardo Keisuke Matsushita Jennie Zheng
Uniaxial Tension and Compression Testing of Materials Nikita Khlystov Daniel Lizardo Keisuke Matsushita Jennie Zheng 3.032 Lab Report September 25, 2013 I. Introduction Understanding material mechanics
More informationStrip Flatness Prediction in a 4 High Tandem Mill Using a Dynamic Model.
Strip Flatness Prediction in a 4 High Tandem Mill Using a Dynamic Model. M. A. BelloGomez 1, M. P. GuerreroMata 1, L. A. Leduc Lezama 1, T. P. Berber Solano 1, L. Nieves 2, F. Gonzalez 2, H. R. Siller
More informationSimulation of Residual Stresses in an Induction Hardened Roll
2.6.4 Simulation of Residual Stresses in an Induction Hardened Roll Ludwig Hellenthal, Clemens Groth Walzen Irle GmbH, NetphenDeuz, Germany CADFEM GmbH, Burgdorf/Hannover, Germany Summary A heat treatment
More informationCapturing complex nonlinear structural response through a series of linear analyses
Capturing complex nonlinear structural response through a series of linear analyses Supervisors: prof.dr.ir. Jan G. Rots dr.ir. Max A. N. Hendriks 1 BACKGROUND Reasons of research: Underground construction:
More informationANALYSIS OF GASKETED FLANGES WITH ORDINARY ELEMENTS USING APDL CONTROL
ANALYSIS OF GASKETED FLANGES WITH ORDINARY ELEMENTS USING AP... Page 1 of 19 ANALYSIS OF GASKETED FLANGES WITH ORDINARY ELEMENTS USING APDL CONTROL Yasumasa Shoji, Satoshi Nagata, Toyo Engineering Corporation,
More informationFatigue. 3. Final fracture (rough zone) 1. Fatigue origin. 2. Beach marks (velvety zone)
Fatigue Term fatigue introduced by Poncelet (France) 1839 progressive fracture is more descriptive 1. Minute crack at critical area of high local stress (geometric stress raiser, flaws, preexisting cracks)
More informationDESIGN AND ANALYSIS OF BRIDGE WITH TWO ENDS FIXED ON VERTICAL WALL USING FINITE ELEMENT ANALYSIS
International Journal of Civil Engineering and Technology (IJCIET) Volume 7, Issue 2, MarchApril 2016, pp. 3444, Article ID: IJCIET_07_02_003 Available online at http://www.iaeme.com/ijciet/issues.asp?jtype=ijciet&vtype=7&itype=2
More informationBEHAVIOR OF WELDED TSTUBS SUBJECTED TO TENSILE LOADS
BEHAVIOR OF WELDED TSTUBS SUBJECTED TO TENSILE LOADS R.A. Herrera 1, G. Desjouis 2, G. Gomez 2, M. Sarrazin 3 1 Assistant Professor, Dept. of Civil Engineering, University of Chile, Santiago, Chile 2
More information